Wet-Environment-Induced Structural Alterations in Single- and Polycrystalline LLZTO Solid Electrolytes Studied by Diffraction Techniques
Redhammer, Günther J.; Badami, Pavan; Meven, Martin; Ganschow, Steffen; Berendts, Stefan; Tippelt, Gerold; Rettenwander, Daniel; ACS Applied Materials & Interfaces  (2020) –; doi:10.1021/acsami.0c16016

data_4518361
_publ_section_title
;
 Wet-Environment-Induced Structural Alterations in Single- and
 Polycrystalline LLZTO Solid Electrolytes Studied by Diffraction
 Techniques
;
_journal_name_full               'ACS Applied Materials &amp; Interfaces'
_journal_paper_doi               10.1021/acsami.0c16016
_journal_year                    2020
_chemical_formula_moiety         'Li6  O12  Ta1  Zr0  La3'
_chemical_formula_sum            'La3 Li6.27 O12 Ta1.09 Zr0.91'
_chemical_formula_weight         932.8
_space_group_IT_number           230
_space_group_name_Hall           '-I 4bd 2c 3'
_space_group_name_H-M_alt        'I a -3 d'
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      230
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.5
_audit_creation_date             2019-03-09T18:44:00-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.8775(2)
_cell_length_b                   12.8775(2)
_cell_length_c                   12.8775(2)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    300(1)
_cell_measurement_theta_max      39.99
_cell_measurement_theta_min      4.33
_cell_measurement_wavelength     0.793
_cell_volume                     2135.48(6)
_computing_cell_refinement       'Bruker APEX2 (Bruker, 2012)'
_computing_data_collection       'Bruker APEX2 (Bruker, 2012)'
_computing_data_reduction        'Bruker APEX2 (Bruker, 2012)'
_computing_molecular_graphics    'Ortep for Windows (Farrugia, 2012)'
_computing_publication_material  'WinGX publication routines (Farrugia, 2012)'
_computing_structure_refinement  'SHELXL (Sheldrick, 2015)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      300(1)
_diffrn_detector_type            CCD
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Huber Eulerian Cradle'
_diffrn_measurement_method
'rotation, \w-scans at 4 different \f positions'
_diffrn_radiation_monochromator  'Ge 422'
_diffrn_radiation_probe          'MLZ SR9B (hot source)'
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     0.793
_diffrn_reflns_av_R_equivalents  0.0278
_diffrn_reflns_av_unetI/netI     0.0637
_diffrn_reflns_Laue_measured_fraction_full 1
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       1
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            674
_diffrn_reflns_point_group_measured_fraction_full 1
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        28.411
_diffrn_reflns_theta_max         39.899
_diffrn_reflns_theta_min         4.325
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.034
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    5.803
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       box-shaped
_exptl_crystal_F_000             3215
_exptl_crystal_size_max          2.35
_exptl_crystal_size_mid          2.15
_exptl_crystal_size_min          1.95
_refine_diff_density_max         0.388
_refine_diff_density_min         -0.486
_refine_diff_density_rms         0.116
_refine_ls_extinction_coef       0.0076(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.01
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     32
_refine_ls_number_reflns         401
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.007
_refine_ls_R_factor_all          0.0642
_refine_ls_R_factor_gt           0.0259
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     'w=1/[\s^2^(Fo^2^)] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0282
_refine_ls_wR_factor_ref         0.0328
_reflns_Friedel_coverage         0
_reflns_number_gt                291
_reflns_number_total             401
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            am0c16016_si_002.cif
_cod_data_source_block           CZ-LLZTO_T=300K
_cod_original_cell_volume        2135.48(10)
_cod_database_code               4518361
_shelx_shelxl_version_number     2014/7